context: The electrode pastes were composed of active materials/carbon black/gel electrolyte precursor whose composition ratios were 60/8.5/31.5 (w/w/w) for the LiCoO2 (LCO) cathode and 52/7.5/40.5 (w/w/w) for the Li4Ti5O12 (LTO) anode, respectively. The gel polymer electrolyte precursor was prepared by mixing a UV-curable ethoxylated trimethylolpropane tri-acrylate (ETPTA) monomer (Aldrich) (including 1.0 wt% 2-hydroxy-2-methl-1-phenyl-1-1propanone (HMPP) as a photo-initiator) and high boiling point electrolyte (1 M LiPF6 in ethylene carbonate(EC)/propylene carbonate(PC) 1/1 (v/v)) in a composition ratio of 15/85 (w/w). To fabricate the bQSSB with cSiPV, the LTO anode paste was directly stencil-printed onto an Al current collector of the cSiPV module without any processing solvents and then exposed to UV irradiation. UV irradiation was performed using an Hg UV-lamp (Lichtzen) with an irradiation peak intensity of approximately 1260 mW cm−2. Subsequently, on the LTO anode (thickness = 50 μm and mass loading = 5.9 mg cm−2), a composite polymer electrolyte (CPE, gel electrolyte precursor/Al2O3 nanoparticles (average particle size ∼300 nm) = 56/44 (w/w)) was introduced through the UV curing-assisted printing process. Then, the LCO cathode paste was stencil-printed directly on the CPE/LTO anode and solidified by UV irradiation, yielding the printed LCO cathode (thickness = 30 μm and mass loading = 6.2 mg cm−2). After placing an Al current collector on top of the printed LCO cathode/printed CPE/printed LTO anode, the QSSB unit cell was obtained. Another QSSB unit cell was introduced, using the same printing process, on the top of the pre-fabricated QSSB unit cell, leading to the bQSSB with a bipolar structure. The number of QSSB unit cells on the cSiPV module was determined from the Vmax of the module concerning the voltage matching between the cSiPV and the bQSSB. Finally, the encapsulation of the bQSSB was conducted with Al pouch packaging substances and a UV-curable hydrophobic polymer (PRO-001, Novacentrix). All assembly steps of the cells were performed in a dry room.
answer:  LiCoO2 (LCO) 